Here is an example of our lab firing schedule for cone 10 oxidation (which the cone-fire mode does not do correctly). We need it to actually go to cone 10, the only way to do that is verify with a cone (self supporting cones are the only accurate way). Then make a note in the record for that schedule in your account at insight-live.com.
Most low-fire bodies contain talc. It is added for the express purpose of increasing thermal expansion. The natural quartz particles present do the same. These are good for glaze fit but bad for ware like this. There are also sudden volume changes associated with cristobalite, but it forms (from quartz) at stoneware temperatures so should not be a concern in terra cotta. You could fiddle with the clay recipe or change bodies, but better to change the firing schedule. While stoneware dunting happens between 950-1150F on the way down, this could be happening anywhere. A simple fix is to slow down the entire cooling cycle. Learn to program your kiln. Use a conservative cooling rate of about 200F/hr (even slower at 1150-950F). No electronic controller? Learn a switch-setting-schedule to approximate this down-ramp (buy a pyrometer if needed).
In ceramics kilns the firing schedule of a kiln is typically managed automatically by an electronic device called a kiln controller. These are especially common on electric kilns.
Devices that melt and bend in a ceramic kiln at specific temperatures. By viewing them through a peephole the operator can tell accurately what temperature the kiln has reached.
Designing a good kiln firing schedule for your ware is a very important, and often overlooked factor for obtained successful firings.